Coloured Gold Alloys
Cristian Cretu and Elma van der Lingen Mintek, Private Bag X3015, Randburg 2125, South Africa
Dedicated to the memory of William S Rapson Received 7 September 1999 From ancient times, gold has been used mostly in decorative items, and the colour of gold plays an important role in this application field. Different methods have been developed to objectively characterize the colour. This paper describes the CIELAB system, which has gained acceptance as an effective way to assess colour. The different coloured gold alloys known today are also described, with emphasis on the relationship between their metallurgy and their colour.
The history of gold goes hand in hand with the 30wt%Au, was used during the time of the Chimu evolution of human civilization, influencing its Empire (ca 1300 AD) by goldsmiths in what is today extension and development ever since the first gold northern Peru (3). Today, various coloured gold alloys item was created. The rich yellow colour of gold has are available, giving the opportunity of creating unique always been attractive to mankind, and gold has been jewellery and decorative items (Figure 1). used in all parts of the world, since as far back as 3000 It is the intention of this paper to briefly review the BC (1, 2). formation of, and assessment of, colour in metals, as well Gold and copper are the only two metals that as the different coloured gold alloys and their properties. exhibit colour. Owing to this property, gold alloys can be made to assume a range of colours by varying the alloying additions. In 862 BC the Lydians were using coins made of a green gold-silver alloy known as FORMATION OF COLOUR IN ‘electrum’ and composed of 73wt%Au and 27wt%Ag. METALS A red gold alloy, the combination of 70wt%Cu with We perceive colour when the different wavelengths composing white light selectively interfere with matter by absorption, diffraction, reflection, refraction or scattering, or when a non-white distribution of light has been emitted by a system (4). The wavelength of visible light is of the order of 380-780 nm. Figure 2 shows the energy of the visible spectrum. The formation of colour in metallic elements and their alloys can be explained by means of the band theory. When metal and light interact, electrons from the metal surface situated either below or on the Fermi level absorb photons and enter an excited state on or above the Fermi surface respectively (5). The efficiency of the absorption and re-emission of light depends on the atomic orbitals from which the energy band originated (4). A white reflected light will result if the different colours in white light are reflected equally Figure 1 Jewellery pieces produced by using coloured gold alloys. well. In the case of gold and copper, the efficiency By courtesy of Jenna Clifford decreases with increasing energy, resulting in yellow
Gold Bulletin 1999, 32(4) 115 reflectivity exhibited by fine gold for the low energy Energy Colour Wavelength Frequency part (below 2.3 eV) of the visible spectrum (6) (Figure 14 (Electron Volts) (Nanometers) x 10 (Hertz ) 2). This means that the yellow colour of gold is formed by a selective reflection of the red-yellow wavelengths. 5 250 12 As the silver content increases, a higher reflectivity is displayed for the high energy part of the visible spectrum. Silver has a very similar electronic structure 300 10 4 to that of gold, but the transition of electrons above the Fermi level requires energy in excess of that of the violet end of the visible spectrum, and thus all the 8 400 visible spectrum is reflected, resulting in the 3 characteristic white metallic colour (6).
2 600 COLOUR MEASURING SYSTEMS 700 4 In some applications of gold, mostly in jewellery and Increasing Energy 1000 dentistry, the colour plays an important role. For a very 1 long time, the colour was estimated visually by the 2 2000 producer, but this is no longer appropriate, as the human eye is subjective. There are cases when the 10.000 0 0 colour is the sine qua non condition, as when selecting a solder for repairing a jewellery item. Such repairs and Figure 2 Wavelengths in the visible spectrum. today’s mass produced jewellery both require an objective way of measuring colour. Even small and reddish colours due to the reduction in reflectivity variations in the colour of similar items are a sign of at the blue end of the spectrum. non-professionalism and poor quality, and can be very Measurements performed on gold alloys with costly for jewellery manufacturers. various amounts of silver (Figure 3) show a high The need for accurate colour measurement led to the creation of different systems designed to assess the colour. The Munsell system describes the colour by 100 using three co-ordinates: ‘hue’, ‘chroma’ and ‘value’ (7). The ‘hue’ is the colour name described in words (red, 5 green, blue, etc.), ‘chroma’ denotes the intensity of the 80 colour as the separation from a white-grey-black axis, and the ‘value’ describes the position on the white-grey- 4 3 black scale. The Munsell system still relies on the human 60 eye, and colours are described by visually comparing 2 them with standard files and finding the closest match. However, the jewellery industry requires a system 1 40 whereby a reference point for colour can be established in order to have uniformity between the various Reflectivity Percent manufacturers. The DIN system used as the European 20 reference for gold colour is based on physical colour Visible spectrum comparison with a standard gold panel. Drawbacks of this system are that colour identification still depends on the eye, and lower caratage gold panels are subject 1 2345 Energy of incident light (eV) to discolouration due to tarnishing with time. The Manufacturing Jewellers & Silversmiths of Figure 3 Reflectivity as a function of energy of the incident America’s Committee for Color References has brought light. 1 - fine gold, 2 - Ag50at%Au, 3 - Ag10at%Au, out a Gold Color Reference Kit that is based on the 4 - Ag5at% Au, 5 - fine silver (6). CIELAB system (8, 9). This system offers the
116 Gold Bulletin 1999, 32(4) L spectrum, while the b* co-ordinate measures the WHITE intensity of the blue (negative) or yellow (positive) component. The colour of a sample can be defined by plotting these co-ordinates as a point in the three- dimensional space depicted in Figure 4. The values of L*, a* and b* of a sample are +b obtained as direct readings from a spectrophotometer -a +a which is connected to a computer. The -b spectrophotometer has a resolving power between five and ten times greater than the human eye (7, 10). As the colour of a sample depends on the illuminant, the sample itself and the observer, the spectrophotometer uses an artificial light source that simulates natural light, an array of photodiodes, and the computer as the BLACK observer. Different problems related to measuring colour such as objectivity, accuracy and reproducibility Figure 4 The L*, a*, b* three-dimensional coordinate system. are resolved by this system. advantage of describing colour mathematically without Colour Measurements the intervention of the human eye, and forms part of Figure 5 shows the a* and b* colour co-ordinates of the American Society for Testing and Materials various coloured gold alloys. Their compositions are standard on colour and appearance. CIELAB is an listed in Table 1. internationally recognized colour measurement system The colour difference can also be a measure of the that was developed by CIE (the International tarnishing of an alloy. By calculating the distance Commission on Illumination) and adopted in 1976. between two points in the CIELAB system, the The CIELAB method expresses the colour as difference in colour can be numerically described. The three-dimensional co-ordinates: L*, a*, and b*, where DE* value represents this distance and can be L* is the luminance (brightness) (10). An L* value of 0 calculated (11) with the formula: means that no light is reflected by the sample, and an 1 2 2 2 /2 L* value of 100 means that all incident light is DE* = [(L*2 - L*1) + (a*2 - a*1) + (b*2 - b*1) ] (1) reflected. The a* co-ordinate measures the intensity of the green (negative) or red (positive) component of the
Table 1 Compositions of Coloured Gold Alloys (wt%)
Alloy Au Ag Cu Al Fe In Co 1N-14* (9) 58.5 26.5 15.0 - - - - 2N-18* (9) 75.0 16.0 9.0 - - - - 3N* (9) 75.0 12.5 12.5 - - - - 4N* (9) 75.0 9.0 16.0 - - - - 0N**(9) 58.5 34.0 7.5 - - - - Red gold 50.0 - 50.0 - - - - Blue gold 75.0 - - - 25.0 - - Blue gold 46.0 - - - - 54.0 - Purple gold 80.0 0 - 20.0 - - - Black gold 75.0 - - - - - 25.0 * Standards common to Germany, France and Switzerland ** Standards common to Germany and France
Gold Bulletin 1999, 32(4) 117 40 COLOURED GOLD ALLOYS yellow 35 Pure Gold Alloying additions to gold and copper can create 30 2N-18 various colours, resulting in diversity in jewellery 25 3N applications. It is less well known, however, that gold Red gold 20 1N-14 0N 4N alloys can have colours which are surprisingly different 15 Copper to the conventional alloys, as in the case of blue, black 10 Blue gold (Fe) or purple gold alloys (Figure 7). In this paper coloured b* co-ordinate 5 Silver gold alloys are classified in the following three main Black gold 0 metallurgical categories: Blue gold Purple gold blue -5 (In) -10 Au-Ag-Cu System -5 0 5 10 15 20 Intermetallic compounds a* co-ordinate Surface oxide layers. green red Au-Ag-Cu System Figure 5 CIELAB co-ordinates of various coloured gold alloys. The Au-Ag-Cu system is the basis of the most common gold jewellery and dental alloys used today, The subscripts 1 and 2 refer to the co-ordinates of and dates back several millennia. Colour variations of the initial and the tarnished sample respectively; L*, a* and b* were defined above as being the CIELAB colour co-ordinates of the respective alloys/samples - see text near Figure 4. The DE* described the distance between two points representing the colour of the samples in the tridimensional CIELAB system. By plotting the DE value versus the heat treatment time, the colour change can be visualized in a graph such as the one in Figure 6. In this case, the tarnish behaviours of two gold alloys are compared with a standard one.
70 Alloy 2 60 Standard alloy 50 Alloy 1 40
30 DE Values
0 0 50 100 150 Heat Treatment Duration (min)
Figure 6 Colour differences of three alloys after the same heat Figure 7 Pendant produced with 18 ct yellow, white and purple treatment in air. The closer the curves are to the gold, Sandawana emeralds and diamonds. Courtesy of standard, the smaller the colour difference. Hans Meevis, Serol-Wana Studio, Botswana.
118 Gold Bulletin 1999, 32(4) yellow, red and green can be obtained by different state above the Fermi level. The wider the gap, the ratios of Au:Ag:Cu. Figure 8 illustrates the rich, yellow higher the energy absorbed from the incident light, colour of high carat gold. White gold is also based on and therefore the reflectivity increases not only for the the Au-Ag-Cu system, and the white colour results red and yellow regions of the spectrum, but also for the from alloying with elements known for their bleaching green (6). characteristics, such as nickel (Ni), palladium (Pd), and The metallurgy of the ternary Au-Ag-Cu system, manganese (Mn). Alloying additions to the ternary including the order-disorder phenomena, has been system are also used to improve properties like extensively studied, and reviewed in-depth by Prince castibility and hardness. et al (13), Rapson (14, 15), and Yasuda (16). An example of a green gold item is shown in Figure 10.
Figure 8 Items produced with hard 24 carat gold revealing the rich, yellow colour of the metal. Figure 10 Green gold elephants donated to ‘The Three Tenors’ Yellow, Green and Red Gold Alloys by Sarah Da Vanzo of Consolidated Bullion Ltd, A multitude of hues and colours can be obtained in the South Africa. Au-Ag-Cu system alone by variation of composition as shown in the ternary phase diagram in Figure 9. Zinc (Zn) additions of up to 15wt% can be added Additions of copper give a reddish tint to the alloy, and to alloys of the Au-Ag-Cu system to change the red additions of silver make the alloy greenish. In colour of copper-rich alloys to reddish yellow or dark accordance with band theory, the addition of silver to yellow (17). These alloys are characterized by good the Au-Cu alloy causes a widening of the energy gap workability. Zinc additions affect both AuCu ordering ␣ ␣ that the electrons have to overcome to reach an energy and the extent of the two phase 1 + 2 region and, therefore, affect the age-hardening characteristics of the alloys (17, 18). A relationship between the Au RY-Red Yellow composition and colour was developed for 14 carat 90 10 RY GY-Green Yellow alloys containing zinc (19). After many colour 80 measurements, a colour index was designed, which can 20 18 Ct. 70 be calculated from the weight percentages of silver, 30 Yellow GY Gold Weight % 60 14 Ct. copper and zinc using the following formula: 40 50 50 10 Ct. 40 60 Cu Yellowish Greenish
Yellowish ______30 Colour index = (2) Copper Weight % Red 70 Ag + 2 Zn 20 80 Whitish 10 90 Cadmium (Cd) additions of up to 4wt% have also Reddish been used for the production of 18 carat green alloys. Cu 10 20 30 40 50 60 70 80 90 Ag 75Au-23Cu-2Cd results in a light green alloy, and Silver Weight % 75Au-15Ag-6Cu-4Cd is the composition of a dark Figure 9 Relationship between colour and composition in the green alloy (20). Cadmium is mostly known as an ternary Au-Ag-Cu system (12). alloying element used for production of solders.
Gold Bulletin 1999, 32(4) 119 However, CdO is considered very toxic, being an irritant to the respiratory system, causing irreversible damage to the kidney, and is classified by the International Agency for Research in Cancer as a carcinogen (21 - 23).
White Gold White gold alloys were originally developed as substitutes for platinum, and are commonly used in the jewellery industry for diamond setting, combination white/yellow jewellery items, and clasps (electroplated with yellow gold) for high-quality collars due to their high strength (Figure 11). These alloys have been used less than the coloured gold alloys in the past, but fashion trends and the increase in the gold price in 1972-1973, Figure 11 White gold and combination white/yellow gold brought silver jewellery and white gold into prominence jewellery designed by Jenna Clifford, South Africa. (24). In Europe, a new trend towards more white gold jewellery has recently become apparent. effect. In the gold-copper-nickel-zinc alloys, nickel is The white gold alloys used in the jewellery industry the primary bleaching agent, and zinc is used as are based primarily on Au-Cu-Ni-Zn, and Au-Pd-Ag secondary bleacher to compensate for the colouring combinations. The bleaching effect of nickel or effect of copper. Nickel-containing white gold alloys palladium is a result of lowering the reflectivity of the are characterized by their high as-cast hardness, rapid alloy for the low energy part of the visible spectrum. work hardening and tendency to fire-cracking. The Absorption processes become possible at energies commercial alloys undergo separation into gold-rich considerably lower than for pure gold, and the (Au-Cu) and nickel-rich (Ni-Cu) phases, which reflectivity is reduced in the red and infrared regions of produces considerable hardness (25). As these alloys the spectrum (6). Figure 12 shows the reflectivity curves have poor formability, frequent intermediate annealing for different nickel and palladium-containing alloys. treatments are required (26). Copper is added to Nickel has traditionally been used for white gold improve plasticity and workability. The use of nickel- alloys because of its low cost and strong bleaching containing gold alloys in the jewellery industry has
100 100 2 1 1 3 2 4 80 80 5 5 3 4 6
40 40 Reflectivity Percent Reflectivity Percent
20 20 Visible spectrum Visible spectrum
1 2345 1 2345 Energy of incident light (eV) Energy of incident light (eV) Figure 12 Reflectivity curves for Ni-(left) and Pd-(right) containing gold alloys (6). Left: 1 - fine Au, 2 - Au2at%Ni, 3 - Au5at%Ni, 4 - Au10at%Ni and 5 - pure Ni. Right: 1 - fine Au, 2 - Au5at%Pd, 3 - Au10at%Pd, 4 - Au20at%Pd, 5 - Au30at%Pd and curve 6 - pure Pd
120 Gold Bulletin 1999, 32(4) become less popular, due to the allergic reaction caused Primary requirements desirable in white gold alloys by nickel when in contact with the skin (27). include (32): Comparison between the properties, advantages Suitable white colour and high reflectivity and disadvantages of nickel- and palladium-containing A reasonable hardness in the as-cast and annealed white gold alloys has received considerable attention in states (arbitrarily <200 VH) the literature (28 - 31). The palladium-containing Adequate cold workability/formability (arbitrarily white gold alloys are characterized by low as-cast >25% elongation) hardness, excellent ductility and cold working A relatively low liquidus temperature (arbitrarily properties, good colour match with sufficient <1100°C) palladium additions, and no tendency to fire-cracking. Cost-effective alloying elements The colour of the Au-Pd alloys ranges from yellow A considerable amount of work has been done to gold to white after the palladium content reaches identify alloying elements that would yield the 15wt%. However, palladium-containing gold alloys are desired combination of properties required for an unattractive due to their high liquidus temperature and ideal white gold alloy. Table 2 summarizes the high density, and in particular because of the bleaching effects that different alloying elements have increasing cost of palladium. on gold.
Table 2 Potential Alloying Elements for White Gold Alloys and Indications of their Bleaching Effects (27 - 29, 32, 33).
Element Effect Comments Colour Workability Ag Moderate bleach Excellent Sulfur tarnishing, bleaches only low caratage alloys Cu Too red (more than 3%) Improves workability - Co Very slight bleach (1.5%) Excellent Increases liquidus, hardness, allergen Cr Excellent bleach (13%) Impossible 2% Cr has no colour influence; increases solidus temperature above 1100°C Fe Nearly complete Poor to Poor corrosion resistance; increases solidus temperature bleach (16%) satisfactory in combination with 4-5wt% Pd, when more than 10wt% causes excessive hardness and oxidation during lost-wax casting In Moderate bleach (5.5%) Impossible 2% has no colour influence, lowers hardness Sn Moderate bleach (5%) Impossible Embrittlement Zn Moderate bleach (6%) Brittle (more than 6%) Volatile, unsuitable for casting, increases tendency for fire- -cracking, high proportions can cause sensitivity, less than 2wt% improves the lost-wax casting behaviour but still without fully satisfactory results Al Very slight bleach (1.5%) Poor Strong oxide former Mn None (1.5%) Poor Strong oxide former, high reactivity when more than 10wt%, appreciable whitening effect especially in combination with Pd, susceptibility to stress corrosion when used in important quantities Pt Bleaching effect - An expensive precious metal similar to Pd Ti Just perceptible (1.3%) Poor Strong oxide former Nb - - Increases liquidus Ta Just perceptible (7%) Poor Increases liquidus, high reactivity V Strong bleach (25%) Impossible Increases liquidus, toxic, high reactivity
Gold Bulletin 1999, 32(4) 121 Au5Al2, Au2Al, AuAl and AuAl2) develop (15). Studies conducted on bimetallic metal systems revealed that Au2Al and Au5Al2 form first, and that AuAl2 is the final equilibrium phase (35, 36). Differential diffusion rates of aluminium and gold lead to formation of Kirkendall voids causing porosity and, eventually, breakage of the aluminium-gold joint (37). This mechanical failure was nicknamed ‘purple plague’. However, although the purple gold compound is brittle, it is stable and does not disintegrate with heat treatment (38). The Au-Al phase diagram (Figure 14) contains a number of intermetallic compounds formed at compositions situated close to the gold-rich end of the diagram. AuAl2 has a gold content close to that of an 18 carat alloy (75 per cent gold), which makes it possible to produce a hallmarkable 18 carat purple alloy.
Weight Percent Gold 020 5040 60 70 80 90 95 100 1100 1060°C 1064.43°C
800 Figure 13 Purple gold used in a pin. The purple colour is given Al2Au by the AuAl2 intermetallic compound. 700 650°C 625°C 624°C Temperature ° C ␥ AlAu2 Intermetallic Compounds 600 575°C (Au) (Al) 545 545 525 ␤
Purple Gold AlAu ␣ 500 AlAu2 4 ␤ AlAu2
The intermetallic compounds are a special group of AlAu materials with properties very different from the 400 0 10 20 30 40 50 60 70 80 90 100 individual metals that constitute them. An Al Atomic Percent Gold Au intermetallic compound is defined by an intermediate phase in an alloy system, having a narrow range of Figure 14 Au-Al phase diagram (39). homogeneity and relatively simple stoichiometric proportions. They are usually brittle, which makes The microstructure of an 18 carat purple gold their use in traditional jewellery virtually impossible, alloy (Au / 25wt%Al) is shown in Figure 15, where the but can, however, be faceted and used as gemstones or light grey phase represents the purple colour (38). As inlays (Figure 13). the composition deviates from AuAl2 towards the The best known among these compounds is aluminium-rich side of the phase diagram, the colour AuAl2, which is formed at 79wt%Au and 21wt%Al approaches that of aluminium. The volume percentage (34). AuAl2 has a higher melting point than its of the purple intermetallic phase decreases, with an constituents, indicating the compound’s increase in the second-phase consisting of an thermodynamic stability. The compound is aluminium-rich solid solution. When the composition characterized by its beautiful purple colour. deviates from the AuAl2 to the gold-rich side of the The purple gold compound has received phase diagram a new intermetallic compound, AuAl, considerable attention from the microelectronic forms at 88wt%Au content and replaces the AuAl2, industry. If bonds between gold and aluminium in altering the alloy’s colour. The purple colour is electronic devices are heat treated above 250°C, all five preserved until the aluminium content decreases to gold-aluminium intermetallic compounds (Au4Al, 15wt% (40).
122 Gold Bulletin 1999, 32(4) and AuGa2 at 58.5wt%Au. Both have a similar crystal structure to the purple gold compound which is based on the CaF2 prototype. The blue colour is ‘diluted’ in a similar manner to that of purple gold. The intermetallic compounds behave in some ways like pure metals, which makes it possible to calculate their band structures. The reflectivity falls in the middle of the visible spectrum and rises again towards the violet end, giving distinctive colours in each case (43). Figure 19 shows the reflectivity as a function of the energy of the incident light for AuAl2, AuIn2, and AuGa2.
Spangold Certain Au-Cu-Al alloys form an interesting surface texture resulting in a new family of gold alloys known Figure 15 Secondary electron image of as-cast Au-25 per cent Al purple gold (38). Weight Percent Indium 0 2010 30 5040 60 70 80 90 100 1200 The crystal structure of AuAl2 was determined in ° 1934 to be the simple cubic CaF2 structure (Figure 16). 1064.43 C 1000 More recent research (41) revealed that the aluminium L sublattice is incompletely occupied and that the actual 800 composition of AuAl2 is closer to Al11Au6. (Au) 649.25°C 641°C 600 540.7°C 509.6°C Blue Gold ␣ 487 1 457.5 495.4°C ⑀ 482 55.3 Two other intermetallic compounds that are known to 35 454.3°C 400 374.6 ␥ Temperature ° C 337 produce colours in gold alloys are AuIn , which has a ␤ 364.5 2 ⑀1 ␥1 275 224.3°C clear blue colour, and AuGa2 (6), which displays a 39 ° ° 200 8 ~156 C 156.634 C
slight bluish hue. Figures 17 and 18 show the Au-In AuIn
␤ AuIn 1 (In) and Au-Ga phase diagrams. The gold-indium 0 intermetallic compound AuIn2 forms at 46wt%Au, 0 10 20 30 40 50 60 70 80 90 100 Au Atomic Percent Indium In
Figure 17 Au-In phase diagram (39).
Weight Percent Gallium 0 10 20 30 5040 60708090100 1200 1064.43°C 1000 L 800
600 ␣ 491.3°C 1 461.3°C 415.4°C 409.8°C 375 448.6°C 400 (Au) 348°C 348.9 339.4°C 282°C 274 ␥ 286°C Temperature ° C 200 ␤
␤1 ␥1 2 30°C AuGa 0 AuGa 29.7741°C (Ga) -200 0 10 20 30 40 50 60 70 80 90 100 Au Atomic Percent Gallium Gu Figure 16 Crystal structure of CaF2 - prototype for AuAl2, AuIn2 and AuGa2 (42). Figure 18 Au-Ga phase diagram (39).
Gold Bulletin 1999, 32(4) 123 100 observed behaviour can be explained by assuming that the alloys exist in two structures: a high-temperature ordered B2-type phase, which is body-centred cubic, 80 and an ordered phase stable at lower temperatures, which has a body-centred tetragonal structure (46). By cooling the material below 20°C, the high- 60 temperature phase is converted to the structure of the 3 ordered phase irrespective of the cooling rate. The spangling heat treatment is normally conducted by 2 40 heating the item in a bath of hot oil at between 150 and 200°C for 10 minutes and then cooling it to Reflectivity Percent 1 below room temperature.
20 Visible spectrum Surface Oxide Layers The coloured gold materials described above have the common feature of preserving the same colour in cross 1 2345section. In the quest for different colours, another Energy of incident light (eV) technique is used, which involves the formation of a coloured oxide layer on the alloy during heat treatment Figure 19 The reflectivity as a function of the energy of the incident light for the intermetallic compounds: 1 - in air. As gold does not discolour in air, the metal is alloyed with a base metal characterized by a low AuAl2, 2 - AuIn2, 3 - AuGa2 (6). oxidation resistance. The oxide layer is only a surface as ‘Spangold’ (44, 45). Two different colours are film, and has limited thickness, which could result in produced by these intermetallic compounds: a yellow the coloured layer being damaged when used in high 76Au-19Cu-5Al alloy, and a pink 76Au-18Cu-6Al wear applications. Surface oxidation is performed as alloy. The decorative spangling effect is the result of a the final treatment after the article has been buffed and change in the crystal structure which creates many polished. small facets on the previously polished surface (Figure 20). During cooling from the high temperature phase, the alloys undergo a quasi-martensitic transformation, which involves ordering of the atoms and shear. The
Figure 20 An 18 ct dagger, with Spangold blade, finished with red Figure 21 The ‘Hearts’ collection in blue gold by Ludwig ivory wood, rubies, red tourmaline, and yellow gold. Muller, Switzerland.
124 Gold Bulletin 1999, 32(4) Liver of sulfur (potassium sulfide) can be used to colour gold alloys containing a significant quantity of copper (18ct and lower), and a range of colours varying from brown to black can be obtained (20). VA Blue Gold SA of Geneva launched, in 1988, an alloy that turns to a rich sapphire blue with heat treatment at 1800°C (47, 48). The gold, with content between 20 and 23 carat, is alloyed with ruthenium, rhodium and three other alloying elements. The blue surface layer is between 3 and 6 μm in thickness. An 18 carat gold alloy, which consists of 24.4wt%Fe and a maximum of 0.6wt%Ni (49), forms a blue oxide layer on heat treatment in the atmosphere between 450 and 600°C (Figure 21). The oxide layer turns to a blue- green colour with an increase in gold content to 85wt%. Black gold generally contains cobalt, which forms a Figure 23 Secondary electron image of the oxide layer on the black cobalt oxide layer on the surface with heat surface of the Au25wt%Co alloy. treatment between 700 and 950°C (50, 51) (Figure hardening cycle such as that used after the colouring of 22). Other alloying elements also known to give a stainless steel was incorporated (53). The addition of blackish layer on oxidation are copper, iron and chromium results in a thinner oxide layer which titanium. Black gold alloys also contain at least one of consists mainly of Cr2O3 and has an olive-green hue. the platinum-group metals, silver, or nickel. The wear resistance of an Au15wt%Co10wt%Cr was Van Graan and Van der Lingen (52) improved the significantly better than that of a binary Au25wt%Co wear resistance of 18 carat cobalt-containing gold alloy, although the oxide layer was approximately five through chromium additions. An electrolytic times thinner (Figure 23). The microstructure of the alloy in Figure 23 is composed of a gold-rich phase containing ca 94wt%Au and a cobalt-rich phase containing ca 90wt%Co. Between the CoO layer and the matrix, is a cobalt-depleted zone containing only ca 2.4wt%Co, resulting from cobalt segregation to the surface during oxidation.
THE FUTURE OF COLOURED GOLD ALLOYS
Gold jewellery has enchanted people for thousands of years. Hues and colours are only variations on the same artistic theme of beauty and brilliance. Gold will always be distinctive due to its unique yellow colour, but the need for diversity and originality will cause some of the coloured gold alloys to remain in fashion. New designs and ideas will certainly arise, and with today’s knowledge and technologies, new solutions will most likely be found for the challenges posed by some of the coloured gold alloys.
ACKNOWLEDGEMENTS Figure 22 Anne Greenwood, South Africa, used black gold to enhance contrast in a multi-coloured jewellery piece. This paper is published by permission of Mintek.
Gold Bulletin 1999, 32(4) 125 ABOUT THE AUTHORS 20 O. Untracht, in ‘Jewelry Concepts and Technology’, ed. R. Hale, Doubleday & Company, London, 1982, pp. 391, 718 Dr Elma van der Lingen obtained a PhD degree in 21 M. Dabalà, M. Magrini and M. Poliero, Gold Technol., 1998, No. 24, p. 6 1998 from the Department of Metallurgical 22 C.S. Freeman and C.J. Jones, in ‘The Santa Fe Symposium on Jewelry Manufacturing Engineering and Materials Science at the University of Technology 1988’, ed. D. Schneller, Santa Fe, 1989, p. 131 Pretoria. She has been an employee of Mintek for the 23 G. Normandeau, in ‘The Santa Fe Symposium on Jewelry Manufacturing Technology past ten years and is heading the Precious Metals 1988’, ed. D. Schneller, Santa Fe, 1989, p. 179 Group in the Physical Metallurgy Division. 24 W.S. Rapson and T. Groenewald, in ‘Gold Usage’, Academic Press Inc. Ltd., London, Cristian Cretu obtained an MSc degree from the 1978, p. 9 Materials Science and Engineering Faculty of the 25 A.S. McDonald and G.H. Sistare, Gold Bull., 1978, 11, 128 Politechnica University of Bucharest, Romania in 26 M.R. Pinasco and E. Stagno, Gold Bull., 1979, 12, 53 1996. He started working as an engineer for Mintek in 27 P. Bagnoud, S. Nicoud, P. Ramoni, Gold Technol., 1996, No. 18, p. 11 1997 in the Precious Metals Group. He had previously 28 G. Normandeau, Gold Bull., 1992, 25, 94 worked in the Non-Ferrous and Rare Materials 29 G. Normandeau and R. Roeterink, Gold Bull., 1994, 27, 70 Institute in Bucharest, in the Powder Metallurgy 30 C.P. Susz and M.H. Linker, Gold Bull., 1980, 13, 15 Laboratory. 31 I.B. MacCormack and J.E. Bowers, Gold Bull., 1981, 14, 19 32 G.P. O’Connor, Gold Bull., 1981, 11, 35 33 M. Dabala, M. Magrini, M. Poliero and R. Galvani, Gold Technol., 1999, no. 25, p. 29 REFERENCES 34 W.S. Rapson, Gold Bull., 1996, 29, 141 35 T. Inagaki, E.T. Arakawa and T.A. Callcott, J. Appl. Phys., 1981, 52, 5597 1 S. Watanabe, in ‘Precious Metals Science and Technology’, eds. L.S. Benner, T. Suzuki, 36 R. Pretorius, T.K. Marais and C.C. Theron, Materials Science and Engineering, 1993, K. Meguro and S. Tanaka, International Precious Metals Institute, Allentown, 1991, 1 10, 1 2 World Gold Council, Gold Jewellery in the 1990s, Internet, http://www.gold.org/ 37 T. Raymond, Semicond. Int., 1989, 12, 152 Ginfos/Gi5jew.htm, 1999 38 R. Süss and C. Cretu, in ‘MSSA Proceedings’, eds. M. McLean, J.A.A. Engelbrecht, 3 World Gold Council, The New World - Pizzaro and Atahualpa, Internet, J.H. Neethling, C. Dennison, D. Mycock and R.H.M. Cross, Microscopy Society of http://www.gold.org/Ginfos/Gi1anc.htm Southern Africa, Johannesburg, 1998, 28, 20 4 K. Nassau, Colour Res. and Appl., 1987, 12, 4 39 T. Massalski, J. Murray, B. Lawrence, B. Hugh, (eds.), ‘Binary Alloy Phase Diagram’, 5 K. Yonemitsu, in ‘Precious Metals Science and Technology’, eds. L.S. Benner, T. Suzuki, American Society for Metals, Metals Park, Ohio, 1986, 1, 90, 260, 270 K. Meguro and S. Tanaka, International Precious Metals Institute, Allentown, 1991, 40 S. Hori, K. Kurokawa, T. Shimizo, M. Steel, M. Tsuboi and K. Yanagase, in ‘Precious p.13 Metals Science And Technology’, eds. L.S. Benner, T. Suzuki, K. Meguro and S. Tanaka, 6 K.E. Saeger and J. Rodies, Gold Bull., 1977, 10, 10 International Precious Metals Institute, Allentown, 1991, p. 430 7 D.P. Agarwal and G. Raykhtsaum, in ‘The Santa Fe Symposium on Jewelry 41 H. Büchler and K.-J. Range, J. Less-Common Met., 1990, 160, 143 Manufacturing Technology 1988’, ed. D. Schneller, Santa Fe, 1988, p. 229 42 R. Cahn, Nature, 1998, 396, 52 8 M. Plotnick, American Jewelry Manufacturer., Jan. 1991, 20 43 S.S. Vishnubhatla and J.P. Jan, Philos. Mag., 1967, 16, 45 9 G. Raykhtsaum and D.P. Agarwal, Gold Technol., 1997, No. 22, p. 26 44 I.M. Wolff and M.B. Cortie, Gold Bull., 1994, 27, 45 10 R.D. Overheim and D.L. Wagner, in ‘Light and Color’, John Wiley & Sons Inc., New 45 M. Cortie, I. Wolff, F. Levey, S. Taylor, R. Watt, R. Pretorius, T. Biggs and J. Hurly, York, 1982, 63, 253 Gold Technol., 1994, No. 4, p. 30 11 G. Raykhtsaum and D.P. Agarwal, American Jewelry Manufacturer, February 1990, 116 46 F.C. Levey and M.B. Cortie, in ‘Solid-State Phase Transformations ‘99’, 1999, in press. 12 J. Leuser, Metall., 1949, 3, 105 47 C. Kremkov, Jewellery News Asia, June 1988, p. 48 13 A. Prince, G.V. Raynor and D.S. Evans, in ‘Phase Diagrams of Ternary Gold Alloys’, 48 D.M. Lakin, Aurum, 1988, 34, 34 The Institute of Metals, London, 1990, p. 7 49 L. Muller, United States Patent 5,059,255, 1991 14 W.S. Rapson, Gold Bull., 1990, 23, 125 50 K. Nakama, European Patent 438980, 1991 15 W.S. Rapson, in ‘Intermetallic Compounds. Principles and Practice’, eds. J.H. 51 T. Takayanagi, N. Marita and C. Seki, United States Patent 5,139,793, 1992 Westbrook and R.L. Fleischer, John Wiley & Sons, Chichester, 1994, 2, 559 52 L. Van Graan and E. Van der Lingen, in ‘MSSA Proceedings’, eds. M. McLean, J.A.A. 16 K. Yasuda, Gold Bull., 1987, 20, 90 Engelbrecht, J.H. Neethling, C. Dennison, D. Mycock and R.H.M. Cross, Microscopy 17 A.S. McDonald, and G.H. Sistare, Gold Bull., 1978, 11, 66 Society of Southern Africa, Johannesburg, 1998, 28, 19 18 D. Ott, Gold Technol., 1997, No. 22, p. 31 53 T.E. Evans, A.C. Hart and W.H. Sutton, British Patent 47048/72, 1972 19 D.P. Agarval and G. Raykhtsaum, in ‘Precious Metals 1993, Proceedings of the 17th International Precious Metals Conference, Newport, Rhode Island’, ed. R.K. Mishra, International Precious Metals Institute, Newport, Rhode Island, 1993, p. 153
126 Gold Bulletin 1999, 32(4)